Share this document with a friend

25

Transcript

National Aeronautics andSpace Administration

Langley Research CenterHampton, Virginia 23681-2199

NASA/CR-2001-211225ICASE Report No. 2001-28

Piezoelectric Ceramics Characterization

T.L. JordanNASA Langley Research Center, Hampton, Virginia

Z. OunaiesICASE, Hampton, Virginia

ICASENASA Langley Research CenterHampton, Virginia

Operated by Universities Space Research Association

September 2001

Prepared for Langley Research Centerunder Contract NAS1-97046

Report Documentation Page

Report Date 00SEP2001

Report Type N/A

Dates Covered (from... to) -

Title and Subtitle Piezoelectric Ceramics Characterization

Contract Number

Grant Number

Program Element Number

Author(s) T.L. Jordan,Z. Ounaies

Project Number

Task Number

Work Unit Number

Performing Organization Name(s) and Address(es) National Aeronautics and Space Administration LangleyResearch Center Hampton, Virginia 23681-2199

Performing Organization Report Number

Sponsoring/Monitoring Agency Name(s) and Address(es)

Sponsor/Monitor’s Acronym(s)

Sponsor/Monitor’s Report Number(s)

Distribution/Availability Statement Approved for public release, distribution unlimited

Supplementary Notes ICASE Report No. 2001-28

Abstract This review explores piezoelectric ceramics analysis and characterization. The focus is on polycrystallineceramics; therefore, single crystals, polymeric materials and organic/inorganic composites are outside thescope of this review. To thoroughly grasp the behavior of a piezoelectric polycrystalline ceramic, a basicunderstanding of the ceramic itself should not be overlooked. To this end, we have presented a briefintroduction of the history of piezoelectricity and a discussion on processing of the ceramic anddevelopment of the constitutive relations that define the behavior of a piezoelectric material. We haveattempted to cover the most common measurement methods as well as introduce parameters of interest.Excellent sources for more in-depth coverage of specific topics can be found in the bibliography. In mostcases, we refer to lead zirconate titanate (PZT) to illustrate some of the concepts since it is the mostwidely used and studied piezoelectric ceramic to date.

Subject Terms

Report Classification unclassified

Classification of this page unclassified

Classification of Abstract unclassified

Limitation of Abstract SAR

Number of Pages 23

1

PIEZOELECTRIC CERAMICS CHARACTERIZATION

T. L. JORDAN1 AND Z. OUNAIES2

Abstract. This review explores piezoelectric ceramics analysis and characterization. The focus is on

polycrystalline ceramics; therefore, single crystals, polymeric materials and organic/inorganic composites are

outside the scope of this review. To thoroughly grasp the behavior of a piezoelectric polycrystalline ceramic, a basic

understanding of the ceramic itself should not be overlooked. To this end, we have presented a brief introduction of

the history of piezoelectricity and a discussion on processing of the ceramic and development of the constitutive

relations that define the behavior of a piezoelectric material. We have attempted to cover the most common

measurement methods as well as introduce parameters of interest. Excellent sources for more in-depth coverage of

specific topics can be found in the bibliography. In most cases, we refer to lead zirconate titanate (PZT) to illustrate

some of the concepts since it is the most widely used and studied piezoelectric ceramic to date.

Subject classification. Structures and Materials

Key words. piezoelectricity, crystalline ceramic, ferroelectricity, piezoelectric coefficient, hysteresis, poling,

piezoelectric characterization

1. Piezoelectric Materials: History and Processing. Smart materials are materials that undergo

transformations through physical interactions. An alternate definition is that a smart material is a material that senses

a change in its environment and through the use of a feedback system, adapts to correct or eliminate such a change.

Piezoelectric materials, shape-memory alloys, electrostrictive materials, magnetostrictive materials,

electrorheological fluids are some examples of currently available smart materials.

Piezoelectricity stems from the Greek word piezo for pressure. It follows that a piezoelectric material develops

a potential across its boundaries when subjected to a mechanical stress (or pressure), and vice versa, when an

electric field is applied to the material, a mechanical deformation ensues. Piezoelectric materials therefore fall in the

class of smart materials. Ferroelectricity is a subgroup of piezoelectricity, where a spontaneous polarization exists

that can be reoriented by application of an AC electric field.

1.1. Definition and History. Piezoelectricity is a linear effect that is related to the microscopic structure of the

solid. Some ceramic materials become electrically polarized when they are strained; this linear and reversible

phenomenon is referred to as the direct piezoelectric effect. The direct piezoelectric effect is always accompanied by

the converse piezoelectric effect where a solid becomes strained when placed in an electric field. The microscopic

origin of the piezoelectric effect is the displacement of ionic charges within a crystal structure. In the absence of

external strain, the charge distribution within the crystal is symmetric and the net electric dipole moment is zero.

However when an external stress is applied, the charges are displaced and the charge distribution is no longer

symmetric. A net polarization develops and results in an internal electric field. A material can only be piezoelectric

if the unit cell has no center of inversion.

Piezoelectricity is a property possessed by a group of materials, discovered in 1880 by Pierre and Jacques

Curie during their study of the effects of pressure on the generation of electrical charge by crystals such as Quartz,

tourmaline, and Rochelle salt. In 1881, the term "piezoelectricity" was first suggested by W. Hankel, and the

1 M/S 238, NASA Langley Research Center, Hampton, VA 23681. 2 ICASE, M/S 132C, NASA Langley Research Center, Hampton, VA 23681-2199. This research was supported by the National Aeronautics

and Space Administration under NASA Contract No. NAS1-97046 while the second author was in residence at ICASE, NASA Langley Research Center, Hampton, VA 23681-2199.

2

converse effect was deduced by Lipmann from thermodynamics principles. In the next three decades, collaborations

within the European scientific community established the field of piezoelectricity; and by 1910, Voigt’s “Lerbuch

der Kristallphysic” was published and became a standard reference work detailing the complex electromechanical

relationships in piezoelectric crystals [1]. However, the complexity of the science of piezoelectricity made it difficult

for it to mature to an application until a few years later. Langevin et al. [2] developed a piezoelectric ultrasonic

transducer during World War I. Their success opened up opportunities for piezoelectric materials in underwater

applications as well as a host of other applications such as ultrasonic transducers, microphones, accelerometers,

etc…In 1935, Busch and Scherrer discovered piezoelectricity in potassium dihydrogen phosphate (KDP). The KDP

family was the first major family of piezoelectrics and ferroelectrics to be discovered.

During World War II, research in piezoelectric materials expanded to the U.S., the Soviet Union and Japan. Up

until then, limited performance by these materials inhibited commercialization but that changed when a major

breakthrough came with the discovery of barium titanate and lead zirconate titanate (PZT) in the 1940s and 1950s

respectively. These families of materials exhibited very high dielectric and piezoelectric properties. Furthermore,

they offered the possibility of tailoring their behavior to specific responses and applications by the use of dopants.

To date, PZT is one of the most widely used piezoelectric materials. It is noted that most commercially available

ceramics (such as barium titanate and PZT) are based on the perovskite structure (Figure 1). The perovskite structure

(ABO3) is the simplest arrangement where the corner-sharing oxygen octahedra are linked together in a regular

cubic array with smaller cations (Ti, Zr, Sn, Nb etc.) occupying the central octahedral B-site, and larger cations (Pb,

Ba, Sr, Ca, Na etc.) filling the interstices between octahedra in the larger A-site. Compounds such as BaTiO3,

PbTiO3, PbZrO3, NaNbO3 and KNbO3 have been studied at length and their high temperature ferroelectric and

antiferroelectric phases have been extensively exploited. This structure also allows for multiple substitutions on the

A-site and B-site resulting in a number of useful though more complex compounds such as (Ba,Sr)TiO3,

(Pb,Sr)(Zr,Ti)O3, Pb(Fe,Ta)O3, (KBi)TiO3 etc.

Fig 1. Perovskite structure

Starting around 1965, several Japanese companies focused on developing new processes and applications, and

opening new commercial markets for piezoelectric devices. The success of the Japanese effort attracted other

nations, and today the needs and uses extend from medical applications to the communications field to military

applications and the automotive field.

Pb

O

Ti,Zr

3

A review of the early history of piezoelectricity is found in the work of W.G. Cady [3]; and in 1971 Jaffe,

Cook and Jaffe published the book “Piezoelectric Ceramics” [4] that is still one of the most referenced works on

piezoelectricity.

1.2. Piezoelectric Ceramic Processing. The fabrication of most bulk piezoelectric ceramics starts with

powder preparation. The powder is then pressed to the required shapes and sizes, and the green shapes are in turn

processed to mechanically strong and dense ceramics. The more important processes that influence the product

characteristics and properties are powder preparation, powder calcining and sintering. The next steps are machining,

electroding and poling: application of a DC field to orient the dipoles and induce piezoelectricity.

The most common powder preparation is the mixed oxide route. In this process, powder is prepared from the

appropriate stoichiometric mixture of the constituents’oxides. In the case of lead zirconate titanate (PZT): lead

oxide, titanium oxide, and zirconium oxide are the main compounds. Depending on application, various dopants are

used to tailor the properties of interest. PZT ceramics are rarely utilized without the addition of dopants to modify

some of their properties. A-site additives tend to lower the dissipation factor, which affects heat generation, but also

lower the piezoelectric coefficients; for this reason they are mostly used in ultrasonics and other high frequency

applications. B-site dopants increase the piezoelectric coefficients but also increase the dielectric constant and loss.

They are utilized as actuators in vibration and noise control, benders, optical positioning application etc.

Figure 2 shows a flowchart of the mixed oxide route for making PZT ceramics. Mixing of the powders can be

done by dry-ball milling or wet ball milling, both methods having advantages and disadvantages: wet ball-milling is

faster than dry-milling; however, the disadvantage is the added step of liquid removal. The most common method

for making PZT ceramics is through wet-ball milling; ethanol and stabilized zirconia media are added for a wet

milling process. A vibratory mill may be used rather than a conventional ball mill; it was shown by Herner [5] that

this process reduces the risk of contamination by the balls and the jar. Zirconia media are used to further reduce the

contamination risks. The calcination step is a very crucial step in the processing of PZT ceramics; it is important that

the crystallization be complete and that the perovskite phase forms during this step. The goals are to remove any

organics, water or other volatiles left after mixing; to react the oxides to form the desired phase composition before

the ceramic is processed to useful devices; and to reduce volume shrinkage and allow for better homogeneity during

and after sintering.

After calcining, a binder is added to the powder, then the mixture is shaped usually by dry-pressing in a die for

simple shapes, or extrusion, or casting for more complicated bodies. Next, the shapes are sintered: placed in an oven

for binder burn-out and densification.

The major problem in the sintering of the PZT ceramic is the volatility of PbO at about 800°C. To minimize

this problem, the PZT samples are sintered in the presence of a lead source, such as PbZrO3, and placed in closed

crucibles. The saturation of the sintering atmosphere with PbO minimizes lead loss from the PZT bodies. Sintering

can now be carried out at temperatures varying between 1200-1300°C. Despite precautions, there is usually a

resulting loss of 2%-3% of the initial lead content.

After cutting and machining into desired shapes, electrodes are applied and a strong DC field is used to orient

the domains in the polycrystalline ceramic. DC poling can be done at room temperature or at higher temperatures

depending on the material and the composition. The poling process only partially aligns the dipoles in a

polycrystalline ceramic, and the resulting polarization is lower than that for single crystals.

4

Fig 2. Mixed-oxide route of preparing PZT

This processing technique presents many uncertainties and the presence of a wide number of other fabrication

techniques is an indication that there is a great need for the production of reliable PZT ceramics with optimum

properties and microstructure. One problem often encountered is the deviation from stoichiometry. This problem is

often due to impurities present in the raw materials as well as the lead loss during the sintering process, which

invariably results in substantial alterations of the PZT properties. As a result, the elastic properties can vary as much

as 5%, the piezoelectric properties 10% and the dielectric properties 20% within the same batch [6]. Also, the

piezoelectric and dielectric properties generally suffer if there is any lack of homogeneity due to poor mixing. It is

important then that the constituent oxides be intimately mixed. In the method described above, however, the

constituents are solid solutions and it has been shown that an intimate mixing of solid solutions is difficult if not

impossible. More information on the preparation of piezoelectric ceramics can be found in Jaffe, Cook and Jaffe [4],

and Moulson and Herbert [7] among others. Other processing methods including hydrothermal processing and co-

precipitation methods are described in references [8-10]. It is noted that there has been a great deal of development

in powder processing, shaping and sintering [11,12,13] that has resulted in further expanding the application of

piezoelectric ceramics.

1.3. Ferroelectricity. Some piezoelectric materials are also ferroelectric. A ferroelectric material possesses a

spontaneous polarization that can be reversed in direction by application of a realizable electric field over some

temperature range. Most ferroelectric materials have a Curie Temperature, Tc below which they are polar and above

which they are not. The dielectric permittivity often has a peak at Tc and linearly decreases according to the Curie-

Weiss law above it [4,7]. The very large permittivity values that are characteristics of ferroelectric materials are

greatly exploited in many applications, most widely in the multilayer-capacitor industry.

Applying a large alternating electric field causes the polarization to reverse, and this gives rise to the

ferroelectric hysteresis loop, relating the polarization P to the applied electric field E. A typical field-polarization

MIXING of OXIDES: PbO, TiO2, ZrO2

dopants if needed

WET MILLING Zirconia media + Ethanol

24 hrs

DRYING AT 80°C, 12 HRS SIEVING for BETTER MIXING and SIZE REDUCTION

READY for CALCINING

5

loop is illustrated in Figure 3. At large signals, both the electric displacement D and the polarization P are non-linear

functions of the field E. They are related to each other through the linear equation below

iii EPD 0ε+= (1)

where ε0 is the permittivity of free space (=8.85x10-12 C/V-m). For most ferroelectric ceramics, the second term in

equation (1) is negligible, and a D-E loop and P-E loop become interchangeable. Two key characteristics of the P-E

loop are the coercive field Ec and the remanent polarization Pr, both defined by analogy to ferromagnetic materials.

Ec is the field at which the polarization is zero. Pr is the value of the polarization when the electric field is zero.

Once the field is switched off, the material will have a polarization equal to Pr. Once the P-E loop is saturated both

Pr and Ec can be determined. A loop is said to be saturated once the values of Pr and Ec no longer vary.

Fig 3. Hysteresis loop of a poled piezoelectric ceramic

Generally, the existence of the P-E loop is considered as evidence towards establishing that a material is

ferroelectric. A Sawyer-Tower circuit [14] or a modified version of it, is commonly used to obtain a P-E loop. An

AC voltage is applied to the electroded sample; the resulting charge stored on the sample is determined by means of

a large reference capacitor placed in series with the sample. An electrometer can be used to detect the voltage across

the capacitor; by multiplying this voltage with the value of the reference capacitor, the charge across the sample

Pr

Ec

E lectr ic F ie ld

Po

lari

za

tio

n

6

results. The reference capacitor should be 100 to 1000 times the value of the capacitance of the sample. It is noted

that ferroelectric hysteresis loops are both frequency and temperature dependent.

In addition to the P-E loop, polarization switching leads to strain-electric field hysteresis. A typical strain-field

response curve is shown in Figure 4. The shape resembles that of a butterfly, and it is often referred to as the

“butterfly loop”. As the electric field is applied, the converse piezoelectric effect dictates that a strain results. As the

field is increased, the strain is no longer linear with the field as domain walls start switching. For more sources on

ferroelectricity, the reader should consult the bibliography [15-19].

Fig 4. Butterfly loop indicating switching

2. Constitutive Relations and Materials Property. An understanding of piezoelectricity begins with the

structure of the material. To better explain it, let us consider a single crystallite (small single crystal less than 100µm

in average diameter) from a polycrystalline ceramic. This crystal is made up of negatively and positively charged

atoms occupying specific positions in a repeating unit or cell. The specific symmetry of the unit cell determines the

possibility of piezoelectricity in the crystal. All crystals can be divided into 32 classes or point groups (from 7 basic

crystal systems: triclinic, monoclinic, orthorhombic, tetragonal, rhombohedral, hexagonal and cubic). Of the 32

classes, 21 do not possess a center of symmetry, and 20 are piezoelectric (one class, although lacking a center of

symmetry, is not piezoelectric because of the combination of other symmetry elements). The lack of center of

symmetry means that a net movement of the positive and negative ions with respect to each other as a result of stress

Electr ic F ie ld

Str

ain

7

produces an electric dipole. The ceramic, being composed of the random orientation of these piezoelectric

crystallites, is inactive, i.e., the effects from the individual crystals cancel each other and no discernable

piezoelectricity is present. Regions of equally oriented polarization vectors are known as domains. "Poling" is a

commonly used method to orient the domains by polarizing the ceramic through the application of a static electric

field. The electrodes are applied to the ceramic and a sufficiently high electric field is applied such that the domains

rotate and switch in the direction of the electric field. The result is never a full orientation of all domains; however

the polycrystalline ceramic exhibits a large piezoelectric effect. During this process, there is a small expansion of the

material along the poling axis and a contraction in both directions perpendicular to it (see Figure 5). With a large

number of allowable polar directions such as near the morphotropic phase boundary (where the Zr to Ti ratio is

equal to 48 to 52), the maximum deviation of the polar axis of a grain from the average polar direction will be

smaller, and the lowering of the polarization will be minimized assuming optimum alignment.

Fig 5. Poling of a piezoelectric, ferroelectric ceramic

Fig 6. Reference axes

V=0 V=n

3

6

1

4

25

8

2.1. Constitutive Relations. When writing the constitutive equation for a piezoelectric material, account must

be taken of changes of strain and electrical displacement in three orthogonal directions caused by cross-coupling

effects due to applied electrical and mechanical stresses. Tensor notation is first adopted, and the reference axes are

shown in Figure 6.

The state of strain is described by a second rank tensor Sij, and the state of stress is also described by a second

rank tensor Tkl. The relationships relating the stress tensor to the strain tensor, compliance s

ijkl, and stiffness c

ijkl, are

then fourth rank tensors. The relationship between the electric field Ej(first rank tensor) and the electric

displacement Di(also a first rank tensor) is the permittivity ε

ij, which is a second rank tensor. The piezoelectric

equations are therefore written as:

jkijkjTiji TdED += ε

(2)

Sij = dijk Ek + sijklE Tkl (3)

where dijk ,dijk are the piezoelectric constants (third rank tensor). Superscripts T and E denote that the dielectric

constant εij and the elastic constant s

ijkl are measured under conditions of constant stress and constant electric field

respectively. In general, a first rank tensor has three components, a second rank tensor has nine components, a third

rank tensor has 27 components and a fourth rank tensor has 81 components. Not all the tensor components are

independent. Both these relations are orientation-dependent; they describe a set of equations that relate these

properties in different orientations of the material. The crystal symmetry and the choice of reference axes reduce the

number of independent components. A convenient way of describing them is by using axis directions as given by

Figure 6. The convention is to define the poling direction as the 3-axis, the shear planes are indicated by the

subscripts 4, 5 and 6 and are perpendicular to directions 1, 2 and 3 respectively. This simplifies the notations

introduced above, where a 3-subscript tensor notation (i,j,k =1,2,3) is replaced by a 2-subscript matrix notation

(i=1,2,3 and j=1,2,3,4,5,6), and a 2-subscript tensor notation (i,j =1,2,3) is replaced by a 1-subscript matrix notation

(i=1,2,3,4,5,6). A shear strain such as S4 is a measure of the change of angle between the two initially orthogonal

axes in the plane perpendicular to axis 1. The first subscript of the d-constant gives the "electrical" direction (field or

dielectric displacement) and the second gives the component of mechanical deformation or stress. The planar

isotropy of poled ceramics is expressed in their piezoelectric constants by the equalities d32

=d31

(an electric field

parallel to the poling axis 3 interacts in the same way with axial stress along either the 2-axis or the 1-axis) and

d24

=d15 (an electric field parallel to the 2-axis interacts in the same way with a shear in the 2,3-plane as a field along

the 1-axis with a shear in the 1,3-plane). Similar relations hold for the elastic constants because of the isotropy in the

plane perpendicular to the polar axis.

2.2. Property Matrix for a Poled Piezoelectric Ceramic. A piezoelectric ceramic has only one type of

piezoelectric matrix regardless of the symmetry of the constituent crystals. The ceramic is initially isotropic. This

isotropy is destroyed in the poling direction. In the directions perpendicular to the poling direction, the material is

transversely isotropic. The symmetry elements are an axis of rotation of infinite order in the direction of poling and

an infinite set of planes parallel to the polar axis as reflection planes. In crystallographic notation, this symmetry is

described as ∞mm and is equivalent to the hexagonal polar crystal class, 6mm.

The elastic, dielectric and piezoelectric matrices for the cylindrical symmetry of poled PZT are shown in the

equations below. Matrices analogous to the piezoelectric one also apply to other piezoelectric constants such as gij

(described in the next section).

9

s11 s12 s13 0 0 0

s12 s11 s13 0 0 0

s13 s13 s33 0 0 0

0 0 0 s44 0 0

0 0 0 0 s44 0

0 0 0 0 0 2(s11 − s12)

(4)

ε1 0 0

0 ε1 0

0 0 ε3

(5)

0 0 0 0 d15 0

0 0 0 d15 0 0

d31 d31 d33 0 0 0

(6)

For the symmetry of poled ceramics then, the general equations (1) and (2) are replaced by the specific

equations below:

D1 = ε

1 E

1 + d

15 T

5 (7)

D2 = ε2 E2

+ d15 T

4 (8)

D3 = ε

3 E

3 + d

31 (T

1 + T

2) + d

33 T

3 (9)

S1 = s

11

E

T1 + s

12

E

T2 + s

13

E

T3 + d

31 E

3 (10)

S2 = s

11

E

T2 + s

12

E

T1 + s

13

E

T3 + d

31 E

3 (11)

S3 = s

13

E

(T1 + T

2) + s

33

E

T3 + d

33 E

3 (12)

S4 = s

44

E

T4 + d

15 E

2 (13)

S5 = s

44

E

T5 + d

15 E

1 (14)

S6 = s

66

E

T6 (15)

Equations (7)-(9) relate to the direct effect, equations (10)-(15) relate to the converse effect.

10

3. Piezoelectric Parameters: Definitions and Characterization. The parameters that are of interest when

considering the electromechanical effects of piezoelectric materials are the piezoelectric charge coefficients (d31

and

d33

), the piezoelectric voltage coefficients (g31

and g33

) and the piezoelectric coupling factors (k31

, k33

, kp and k

t). The

d-coefficient is the proportionality constant between electric displacement and stress, or strain and electric field

(equations (2) and (3)). High d-coefficients are desirable in materials utilized as actuators, such as in motional and

vibrational applications. The g-coefficient is related to the d-coefficient by the following expression:

dmi = εnmT gni (16)

where m,n =1, 2, 3 and i = 1, 2, ...6. High g-coefficients are desirable in materials intended to be used as sensors, to

produce voltage in response to mechanical stress.

The piezoelectric coupling factor k is a measurement of the overall strength of the electromechanical effect.

It is often defined as the square root of the ratio of electrical energy output to the total mechanical energy input (in

the case of the direct effect) or the mechanical energy available to the total electrical energy (in the case of the

converse effect). The value of k is of course always less than unity because energy conversion is always incomplete.

Other important properties of PZT are the dielectric properties, namely the dielectric constant ε (F/m) and

the dissipation factor or loss tangent tanδ. The dielectric constant is a measure of the charge stored on an electroded

material brought to a given voltage. The dielectric constant of vacuum is ε0=8.85x10

-12 F/m. The relative dielectric

constant K (often referred to as just “the dielectric constant”) is the ratio of ε and ε0, and is dimensionless. In case of

ac field, the dielectric constant has both a real part and an imaginary part; the loss tangent is defined as the ratio of

the imaginary part to the real part.

The values of these constants depend on the PZT compositions. As an example, the d-constants, g-

constants and the dielectric constant for compositions near the morphotropic phase boundary show their highest

values on the tetragonal side of the transition [4]. It is then possible to tune the values of these properties for most

compositions; one way of achieving that is through adding dopants to the PZT formulation.

3.1. Resonant Method and Equivalent Circuit

3.1.1. Resonance method. Any body of mass has certain characteristic frequencies at which it prefers to

resonate. When excited at this resonant frequency, fr, the body will resonate freely with a greater amplitude than at

other frequencies. Following this resonant frequency is an anti-resonant frequency, fa, where the impedance of the

body is at a maximum and the oscillation amplitude is at a minimum. Piezoelectric ceramics are no different and

the measurement of these characteristic frequencies provides the means to evaluate the piezoelectric and elastic

properties of the ceramic. Different modes of vibration of the ceramic, such as thickness or planar, give insight to

the different constants associated with that mode. A typical resonance plot of impedance versus frequency for a

piezoelectric ceramic near a resonance is shown in Figure 7. Notice the resonant frequency, fr, at the point of

minimum impedance and the anti-resonant frequency, fa, at the point of maximum impedance.

11

Fig 7. Impedance of a piezoelectric ceramic at resonance

Fig 8. Resonant equivalent circuit of a piezoelectric vibrator

At resonance, a piezoelectric element may be modeled by the equivalent circuit as shown in Figure 8. This circuit is

commonly referred to as Van Dyke’s Model and is recommended by the IEEE Standard on Piezoelectricity [20]. An

alternate model, proposed by Sherrit et al. [21], eliminates the resistance, R1, and instead represents the remaining

components as complex to better characterize the losses associated with certain piezoelectric elements, especially

polymers. All discussion presented below will assume Van Dyke’s Model. Below fr and above fa, the ceramic

behaves capacitively; however between these two frequencies, the ceramic behaves inductively. This model is only

valid near the resonance. Additionally, the resonance must be sufficiently isolated from other modes to eliminate

the effects of any adjacent modes. To assure isolation of the resonance, sample geometry must be chosen carefully.

Geometries suitable for measuring the different piezoelectric and elastic coefficients are presented in Table 1.

Fixturing of the sample should not impose any constraints on the vibration of the ceramic. This can be

C

LR1

0

1 C1

fr

fa

Imp

ed

an

ce

, Z

F requency, f

12

accomplished by using a point holder positioned at a node of vibration. Also, all leads should be shielded up to the

contact point as much as possible to avoid any stray capacitances which may arise.

Earlier literature has suggested several circuits to measure fr and fa of a piezoelectric ceramic [22-25]. These

circuits usually consist of an oscillator for exciting the sample, a voltmeter or other device for measuring current

through the circuit, and additional discrete components. To find fr, the oscillator is varied in frequency until the

maximum current is detected through the circuit. Similarly, for fa, the frequency of minimum current is determined.

It should be noted that there are actually six characteristic frequencies that may be identified for a particular

resonance which include fm and fn, the frequencies of maximum and minimum impedance; fr and fa, the resonant and

antiresonant frequencies; and fp and fs, the parallel resonant frequency and series resonant frequency. IEEE Standard

177 [23] identifies these six frequencies and establishes that for many cases, including piezoelectric ceramics, one

can make the assumption that fm = fs = fr and fa = fp = fn. For lossy materials, such as some of the piezoelectric thin

films, this assumption can introduce appreciable errors and the six frequencies should be considered separately. The

magnitude of the minimum impedance, Zm, may be determined by substituting an adjustable resistor into the circuit

for the ceramic at the previously identified frequency and adjusting the resistance until the voltmeter reading is the

same as for the ceramic. Today, fully integrated impedance analyzers are commercially available to make this type

of measurement, and even allow the researcher to choose an equivalent circuit model and will report the values of

the discrete components of the equivalent circuit along with fr and fa. Also, commercial off- the shelf software is

now available which can be used in conjunction with an analyzer to evaluate the impedance information and

calculate the relative material properties of a piezoelectric device [26]. These tools can aid the researcher in the

evaluation of material properties, however a basic understanding of piezoelectric behavior is an important

foundation that should not be overlooked.

Table 1.

Sample geometries for measurement of material properties

Dimensional long, slender, length thin, flat plate, thickness poled; thin flat disc, thickness poled

Requirements poled rod; l > 3d l > 3.5 t, w d > 10 t

Properties

Measured

3 33 33

33 33 33

, , tan , ,

, , ,

T D

EM

K k s

s d g Q

δ 3 31 11

11 31 31

, , tan , ,

, , ,

T D

EM

K k s

s d g Q

δ

l

w

t d

tl

d

3 , , ta n ,Tp MK k Qδ

13

3.1.2. Measurement of material properties. Capacitance measurements are usually carried out at 1kHz and at

low excitation voltages (mV level). Although research has shown capacitance and loss to vary with excitation

voltage and frequency [27,28], the 1kHz, low voltage measurement is used in the determination of material

properties. The free relative dielectric constant, KT, is defined as the ratio of the permittivity of the material to the

permittivity of free space. It is calculated from the following:

A

tCK T

0ε= (17)

where t is the distance between electrodes in meters, C is the capacitance in farads, 0ε is the permittivity of free

space (8.85 x 10-12 F/m), and A is the area of an electrode in meters2.

The loss tangent, tanδ, is defined as the ratio of resistance to reactance in the parallel equivalent circuit of

Figure 9a. It is a measure of the dielectric losses in the material and therefore also a measure of the heat generation

capacity of the ceramic when operated under dynamic conditions. This is a direct measurement and is usually

formed at the same conditions as the capacitance measurement.

(a)

(b)

Fig 9. Non-resonant (a) parallel and (b) series equivalent circuit

The three most common coupling coefficients are kp, k31, and k33; where the p is for planar, and the 31 and 33

subscripts are for length extensional and thickness extensional modes. The coefficients k33 and k31 are calculated

from the frequencies of minimum and maximum impedance and are given by the equations

Rp

pC

Rs Cs

14

−+

−

−+

=

r

ra

r

ra

r

ra

f

fff

ff

f

ffk

)(1

2

)(

tan)(

1

2233

ππ

(18)

ψ

ψ+

=1

231k (19)

where:

−

−+=

r

ra

r

ra

f

ff

f

ff

2

)(tan1

2

ππψ (20)

The planar coupling coefficient kp is defined for thin discs and can be approximated by

2

22

r

rap

f

ffk

−≈ (21)

Elastic compliance is the ratio of a material’s change in dimensions (strain) in relation to an externally applied

load (stress). This is the inverse of Young’s modulus. For a piezoelectric material, the compliance depends on

whether the strain is parallel or perpendicular to the poling axis and the electrical boundary conditions. Elastic

constants are calculated from the following equations:

2233 4

1

lfs

a

D

ρ= (22)

233

3333 1 k

ss

DE

−= (23)

2211 4

1

wfs

r

E

ρ= (24)

( )2311111 1 kss ED −= (25)

where ρ is the density of the material in kg/m3 and l is the distance between electrodes and w is the width of the

ceramic. The superscripts D and E stand for constant electric displacement (open circuit) and constant electric field

(short circuit) respectively.

The dij piezoelectric constants, which relate the applied electric field to the strain, can be calculated from the

coupling, elastic coefficients and the dielectric constant. They are ET sKkd 33303333 ε= (26)

ET sKkd 11303131 ε= (27)

The gij piezoelectric constants are related to the dij coefficients by the following equations:

15

TK

dg

30

3333 ε

= (28)

TK

dg

30

3131 ε

= (29)

It should be noted that the piezoelectric coefficients calculated above are only valid at frequencies well below

resonance and do not account for any non-linear behavior of the ceramic.

They are not dependent on the dimensions of the material, however they will vary with the degree of

polarization of the ceramic. They also do not provide the sign of the coefficient, which must be determined through

direct measurements.

The mechanical QM, the ratio of reactance to resistance in the series equivalent circuit of Figure 9a is given by:

−=

22

2

02

1

ra

a

mrM

ff

f

CZfQ

π (30)

3.2. Direct Methods. Direct measurements of the piezoelectric constants are possible and have been used to

quantify the direct and converse effects in ceramic samples. Direct methods are also used to investigate the behavior

of the ceramic in regards to hysteresis, non-linearity, frequency response, aging, thermal behavior, and other

characteristics that are not resolved by the above methods. These methods typically apply a known input to the

ceramic, either an electric field or a force, and record the corresponding output, either a deformation or a charge

under various conditions. These methods are in contrast to the bulk material characterization using the electrical

resonance techniques described above. Many times, the direct measurements are carried out on a ceramic that has

been configured as a sensor or actuator. Typical processing may include electroding, laminating, applying preload,

mounting, and other assembly procedures to be able to effectively adapt the material for use as a sensor or actuator.

These measurements aid the researcher in modeling the behavior of the piezoelectric device and allow the efficient

integration of the devices into real world applications.

Displacement measurements of piezoelectric actuators are performed to determine the magnitude and sign of

the relationship between applied electric field and the strain developed, i.e., the converse effect. For a PZT wafer,

this corresponds to the dij coefficient; however for bending type actuators this relationship does not correlate directly

to any of the measured properties for out of plane bending using the resonance techniques. Based on equations

(10)-(15), it can be seen that for a case where the ceramic is free to expand (Tk = 0), then the strain is only a function

of the product of the applied field Ei and the dij coefficient

iijj EdS = (31)

Careful attention must be paid to the boundary conditions of the ceramic to assure that the above assumption is

valid. In a plot of the strain as a function of applied field, the slope yields an average value of dij. Typically these

measurements are made with a non-contacting displacement transducer [29] to reduce the effects of loading on the

actuator. Laser based and other optical or capacitive displacement measurement techniques are most commonly

used [30-32]. Displacements may range from sub-micron levels for single PZT wafers to the centimeter level for

bending type actuators. For very small displacements, an optical-lever type measurement system or interferometric

techniques [33] have been used to resolve the displacement of the ceramic. Direct application of either foil or

16

optical strain gages has also been utilized for measurement of the actuator strain. These measurements may be made

either statically or dynamically, depending on the measurement system and the intended application of the ceramic.

If dynamic measurements are made, excitation frequencies should be at least an order of magnitude less than any

resonant frequency of the device to assure a linear behavior and that the boundary conditions are suitable for the

intended measurement.

Another direct method used to measure the piezoelectric constants is based on the direct piezoelectric effect

[22,34]. Here, a known load is either applied to or lifted off a ceramic at rest. The resulting charge, which

accumulates on the electrodes, is then measured as a voltage across a capacitor in parallel with the ceramic or the

current from the ceramic can be integrated directly. If Ei is 0 (short circuit), then equation (2) reduces to: Di = dijTj (32)

and knowing the applied stress and measuring the electric displacement, the appropriate dij coefficient can be found.

If a piezoelectric ceramic is immersed in a liquid and the pressure of the liquid is varied, then the piezoelectric

coefficient dh can be quantified by measuring the voltage on a large capacitor in parallel with the ceramic. This

coefficient represents the response of the ceramic to hydrostatic pressure applied equally in all axes. Convention has

dictated that for the dh coefficient, electrodes are perpendicular to the 3-direction. The dh coefficient is related to the

other d coefficients for a ceramic by the equation:

3133 2dddh += (33)

By varying the frequency of the excitation voltage to the ceramic while measuring the displacement, the

frequency response of the device may be obtained. Typical resonant frequencies of bulk ceramic material are in the

kilohertz to megahertz range depending on the mode of vibration, while resonant frequencies of bender types

(unimorph or bimorph) may be less than 100 hertz. For maximum strain, a piezoelectric actuator can be excited at

its natural frequency, however this non-linear behavior must be taken into account if the actuator is to be used over a

range of frequencies. Also, careful attention must be paid to the instrumentation system’s dynamic response, in both

amplitude and phase distortion, when making dynamic measurements. Measurement systems have their own

frequency response characteristics which must be separated from the response of the ceramic under test.

Hysteresis is a phenomenon that is present in all piezoelectric materials. Hysteretic behavior is due to the lossy

nature of the ceramic where the current trails the applied voltage by an angle α related to the loss tangent of the

material. For actuators, this means that the absolute displacement is not only dependent on the excitation voltage

and frequency, but also on whether the voltage is increasing or decreasing. To characterize the amount of hysteresis

in a ceramic, a sinusoidal voltage is applied to the device and the displacement is recorded. By plotting the

displacement vs. driving voltage, as shown in Figure 10, the hysteretic behavior of the ceramic can be observed.

The amount of hysteresis (usually expressed in percent) is defined as the largest difference between the maximum

and minimum displacement for any voltage divided by the total displacement. Of note in Figure 10 is the fact that

as the peak voltage is increased, the amount of hysteresis also increases for any given voltage.

17

Fig 10. Strain hysteresis of a piezoelectric ceramic unimorph

Generally, piezoelectric ceramic actuators exhibit a decrease in their displacement for a given excitation

voltage as they are loaded. This relationship can be seen in equation (3), for the case where Tk ≠ 0. As the load is

increased, the displacement eventually reaches zero and the actuator provides only a force output. This force is

known as the blocked force, and it is the maximum amount of force that the actuator can produce at that voltage. To

characterize this relationship, the actuator is loaded with a load less than the blocked force and the displacement is

measured. If the load is varied, then the force/displacement relationship can be determined (Figure 11). To

determine the blocked force, the actuator must be rigidly held so as not to deform, and the force output measured

with a load cell or other force-measuring device. Because the displacement of some piezoelectric actuators is quite

small, this measurement can be difficult. The blocked force FB can alternately be calculated by the equations below

EB

s

wldEF

33

333= (34)

EB

s

wtdEF

11

313= (35)

where E is the applied field, l, w and t are the length, width and thickness of the ceramic, respectively. Equation (34)

applies to thickness extensional mode and equation (35) applies to length thickness extensional mode.

Actuators with greater displacements better lend themselves to the blocked force measurement (such as domed

pre-stressed actuators or unimorph/bimorph type actuators). The blocked force may also be determined by

extrapolating the force/displacement relationship to zero displacement if a true blocked force measurement is not

practical. In most applications, actuators will operate somewhere between the free (unloaded) state and the

completely constrained state.

-250

-200

-150

-100

-50

0

50

100

150

200

250

-8 -6 -4 -2 0 2 4 6 8

DISPLACEMENT, mils

EX

CIT

ATI

ON

VO

LTA

GE

, vol

ts

18

Fig 11. Typical stress/strain relationship for a piezoelectric ceramic

It has been previously reported that a constant preload applied to a piezoelectric actuator can actually increase

the displacement of the ceramic as compared to an unloaded specimen [34-36]. This may be a result of simply

reducing the compliance or mechanical slop in a PZT assembly or may be a real increase in the d-coefficient. This

effect will reach a maximum and then start to cause a decrease in the coefficient as the pre-load is increased up to

the blocked force.

Temperature effects on the piezoelectric coefficients of ceramics may also be evaluated. Usually, ceramics

must be used well below their Curie temperature to maintain polarization. For hard and soft PZTs, the respective

Curie temperatures are on the order of 360oC (680 oF) and 330oC (626oF). For operation at lower temperatures, even

down to cryogenic levels, the piezoelectric coefficients generally decrease with decreasing temperature. This effect

can be experimentally quantified through either resonance techniques or direct measurements over the desired

temperature range [34].

The power required to drive a piezoelectric ceramic can be calculated from the following equation: 2tan2 rmsVfCP δπ= (36)

when the ceramic is modeled as in Figure 9a where f is the driving frequency, C the capacitance, tanδ the loss

tangent, and Vrms the root mean square of the excitation voltage. Typically, both the capacitance and loss tangent of

the ceramic are assumed to be constant when using equation (36). Doing so can lead to large errors when estimating

the power consumption of a ceramic. To avoid these errors, either the voltage and current supplied to the ceramic

should be measured to provide a direct indication of the power consumption, or the variation of capacitance and loss

of the material as functions of applied field and frequency must be quantified and incorporated into equation (36)

[28]. A number of researchers have investigated the power consumption characteristics of PZT actuators used to

excite a host structure [27,37,38] and found a coupling between the mechanical motion of the structure and the

electrical characteristics of the piezoelectric actuator. Research by Brennan and McGowan [27] shows that the

power consumption of piezoelectric materials used for active vibration control is independent of the coupling effects

of the host structure when the structure is completely controlled. From these findings, they conclude that the power

requirements of the piezoelectric actuator are only dependent upon its geometry and material properties, and the

driving voltage and frequency of the control signal. Research [23] has indicated that both capacitance and resistance

are non-linear functions of the peak amplitude and frequency of the excitation voltage

Increasing applied field

19

With time, piezoelectric effects imparted through poling will degrade. Aging of piezoelectric ceramics, like

many other materials, is logarithmic with time. With most ceramics, a return to initial performance levels can be

accomplished by simply repoling the sample. Aging levels depend on the composition; the coupling coefficient of

soft PZT composition ages at a rate of –1% per time decade versus –2% for a hard composition. Degradation of

piezoelectric behavior also depends on the level of stress to which the ceramic is subjected. Large stress levels can

lead to switching of the polarization and eventually depoling of the ceramic. Large stresses also induce micro

cracking, which can lead to ceramic breakage and failure.

The methods outlined above can be used either separately or together to investigate the dielectric, piezoelectric,

and elastic properties of a ceramic. Resonant techniques, which are the preferred method of measurement of the

IEEE standard, are easy to implement and the associated frequencies can be measured accurately. There is even

commercially available hardware and software available to assist in these measurements and the evaluation of

material properties. However, these methods do not explain any non-linear behavior that is present in the ceramic.

Dependence of material properties on the frequency and amplitude of the applied voltage are among these non-linear

effects. Direct measurements of the piezoelectric constants can quantify the material properties under different

operating conditions and provide insight beyond the standard linear behavior predicted by the resonance techniques.

These methods though, are usually more rigorous in their requirements of material handling and instrumentation.

3.3. Modeling of Piezoelectric Ceramics. There are a host of applications for piezoelectric materials and

despite the fact that they have been studied for over a century, potential for improvement and innovation still

persists. Modeling of piezoelectric ceramics and their properties affords a way to accelerate materials improvement

and aid in device design and development. For that reason, we would be remiss not to mention it, albeit briefly. This

introduction is in no way meant as a comprehensive review of the vast area of modeling of piezoelectricity, however

the references cited provide a good starting place. Care must be taken to differentiate between modeling of the

piezoelectric material and modeling of a “piezoelectric structure”, where often a piezoelectric material is laminated

or adhered to a substrate as a unimorph or bimorph.

A number of researchers experimented with commercial packages such as ANSYS [39]. However, these

commercial packages have limitations. Other groups have written their own codes with varying degrees of success

[40-43]. Finite element schemes combining piezoelectric and acoustic elements proved useful in characterizing the

electromechanical behavior of piezoelectric transducers [44]. Most of these schemes are restricted in that they

assume linearity of the coefficients. Perez et al expanded on these models by including nonlinear elements into the

equivalent circuit [45]. Models of the non-linear hysteretic behavior of piezoelectric materials are abundant in the

literature, and can be divided based on the dimensional scale they probe. Microscopic models primarily stem from

energy relations applied at the atomic or molecular level [46]. Macroscopic models [47-49] often use empirical

relations to describe the behavior of the bulk material. Both methods have their advantages and disadvantages;

microscopic models require a great number of parameters, often not available, and macroscopic models do not

consider the underlying physics. A number of authors proposed a third approach, a meso-scale or semi-microscopic

model that combines the advantages of the previous methods, thus allowing a better way to model the hysteretic

behavior. This is accomplished by starting out from energy principles applied at the microscopic level, then using a

relatively small number of parameters to simulate the behavior of bulk ceramics [50,51].

4. Conclusion. Characterization of the elastic, dielectric and electromechanical properties of piezoelectric

ceramics is crucial for several reasons. First, investigations of the material properties provide a link between the

manufacturing process and ceramic performance. This enables the developer of the materials to adjust the

manufacturing process of the ceramic to produce tailored materials. Second, the engineer can investigate

20

prospective materials for applicability to a specific need. Also, material parameters obtained through

characterization can be used to develop and validate analytical models of the ceramics. Insights gained through

characterization have led to many new devices and uses. For example, investigation of the hydrostatic coefficients

of PZT and those of the piezoelectric polymer polyvinylidene fluoride, PVDF, identified the product of dh and gh as

a figure of merit and led to composite research to combine both materials yielding a superior device that better fits

underwater and hydrophone applications. More than a century after their discovery, piezoelectric ceramics have

become viable for commercial purposes. Researchers continue to diligently uncover novel ways to characterize the

complex electromechanical properties and as they do so, new processing methods and applications are revealed.

Recently, as an example, researchers at MIT have successfully grown piezoelectric single crystals [52], opening

opportunities for newer applications. Published articles on composite processing and characterization have become

more abundant as well.

Without question, piezoelectric ceramics have secured a permanent place in the field of material science and

engineering.

5. Acknowledgement. The authors express their sincere appreciation to Dr. Jeffrey A. Hinkley (NASA Langley

Research Center) for his review of the manuscript and his helpful comments.

5()(5(1&(6

[1] V. W. VOIGT, Lehrbuch der kristallphysik, B. G. Teubner, Leipzig: Berlin, 1910.

[2] °uvres scientifiques de Paul Langevin, Centre National de la recherche scientifique, 1950.

[3] W. G. CADY, Piezoelectricity: An introduction to the theory and applications of electromechanical phenomena

in crystals, Dover Publications: New York, 1964.

[4] B. JAFFE, W. R. COOK, JR. AND H. JAFFE, Piezoelectric ceramics, Academic Press: London, New York,

1971.

[5] S. B. HERNER, The use of acceptor dopants to lower the loss tangent in barium strontium titanate, Thesis:

Pennsylvania State University, 1993.

[6] Measurement of Properties of Piezoelectric Ceramics, Sensor Technology Limited, BM91-309, Manufacturer

Handbook, 1991.

[7] A. J. MOULSON AND J. M. HERBERT, Electroceramics: Materials, properties, applications, Chapman and

Hall: London , New York, 1992.

[8] Q. F. ZHOU, H. L. W. CHAN, AND C. L. CHOY, Nanocrystalline Powder and Fibres of Lead Zirconate

Titanate Prepared by the Sol-Gel Process, Journal of Materials Processing Technology, 63, No. 1-3 (1997),

pp. 281-285.

[9] Z. OUNAIES, Sol-gel and Microwave Processing of PZT Materials for Sensor and Actuator Applications, the

Pennsylvania State University, 1995.

[10] J. P. WHITMAN, Hydrothermal Preparation and Fabrication of Lead Zirconate Titanate (PZT) Ceramics,

the Pennsylvania State University, 1993.

[11] C. NEAR, G. SHMIDT, K. MCNEAL AND R. GENTILMAN, Injection Molded PZT Actuators, SPIE 5th

Annual Symposium on Smart Structures and Materials Proceedings, 3326 (1998), pp. 323-331.

[12] L. M. LEVINSON, Electronic Ceramics: Properties, Devices, and Applications, General Electric Company:

New York, 1988.

[13] ACX Controls Expert, www.ACX.com.

[14] C. B. SAWYER AND C. H. TOWER, Phys. Rev., 35 (1930), pp. 269-273.

21

[15] M.E. LINES AND A. M. GLASS, Principles and Applications of Ferroelectrics and Related Materials,

Clarendon: Oxford, 1979.

[16] Y. XU, Ferroelectric Materials and Their Applications, North-Holland: Amsterdam, 1991.

[17] G. A. SMOLENSKII, V. A. BOKOV, V. A. ISUPOV, N. N. KRAINIK, R. E. PASYNKOV AND A. I.

SOKOLOV, Ferroelectrics and Related Materials, Gordon and Breach Science Publishers: New York,

1984.

[18] J. C. BURFOOT, Ferroelectrics: An Introduction to the Physical Principles, Van Norstrand: London, 1967.

[19] ANSI/IEEE std. 180-1986, IEEE Standard Definitions of Primary Ferroelectric Terms, The Institute of

Electrical and Electronics Engineers, Inc.: New York, 1986.

[20] IEEE Standard on Piezoelectricity, (IEEE Standard 176-1987); Institute of Electrical and Electronic

Engineers, 345 East 47th St, New York, NY 10017.

[21] S. SHERRIT, H.D. WIEDERICK, AND B.K. MUKHERJEE, Accurate Equivalent Circuits for Unloaded

Piezoelectric Resonators, IEEE Ultrasonics Symposium Proceedings, pp. 931-935, 1997.

[22] W. P. MASON AND H. JAFFE, Methods for Measuring Piezoelectric, Elastic, and Dielectric Coefficients of

Crystals and Ceramics. Proceedings of the IRE, 42 (1954), pp. 921-930.

[23] IEEE Standard Definitions and Methods of Measurement for Piezoelectric Vibrators, (IEEE Standard 177-

1966); Institute of Electrical and Electronic Engineers, 345 East 47th St., New York, NY 10017.

[24] K. W. KWOK, H. L. CHAN AND C. L. CHOY, Evaluation of the Material Parameters of Piezoelectric

Materials by Various Methods, IEEE Trans. On Ultrasonics, Ferroelectrics and Frequency Control, 44, No.

4 (1997), pp. 733-742.

[25] Procedures for Measuring Properties of Piezoelectric Ceramics, Morgan Matroc Inc., Technical Publication,

TP-234.

[26] Piezoelectric Resonance Analysis Program, TASI Technical Software, 1996.

[27] M. C. BRENNAN AND A. M. MCGOWAN, Piezoelectric Power Requirements for Active Vibration Control,

SPIE 4th Annual Symposium on Smart Structures and Materials Proceedings, 3039 (1997), pp. 660-669.

[28] T. JORDAN, Z. OUNAIES, J. TRIPP AND P. TCHENG, Electrical Properties and Power Considerations of

a Piezoelectric Actuator, Materials Research Society Symposia Proceedings, 604 (2000), pp. 203-208.

[29] J. T. DAWLEY, G. TEOWEE, B. J. J. ZELINSKI AND D. R. UHLMANN, Piezoelectric Characterization of

Bulk and Thin Film Ferroelectric Materials Using Fiber Optics, MTI Instruments Inc, Application Note,

www.mtiinstruments.com/appnotes/piezo.htm, September 2001.

[30] W. Y. PAN, H. WANG AND L. E. CROSS, Laser Interferometer for Studying Phase Delay of Piezoelectric

Response, Jpn. J. Appl. Phys., 29 (1990), p. 1570.

[31] Q. M. ZHANG, W. Y. PAN AND L. E. CROSS, Laser interferometer for the study of piezoelectric and

electrostrictive strains, J. Appl. Phys., 63 (1988), p. 2429.

[32] T. L. JORDAN, Z. OUNAIES AND T. L. TURNER, Complex Piezoelectric Coefficients of PZT Ceramics:

Method for Direct Measurement of d33, Materials Research Society Symposia Proceedings, 459 (1997), p.

231.

[33] H. D. WIEDERICK, S. SHERRIT, R. B. STIMPSON AND B. K. MUKHERJEE, An Optical Lever

Measurement of the Piezoelectric Charge Coefficient, 8th European Meeting on Ferroelectricity

Proceedings, Nijmegen, The Netherlands, July 4-8, 1995.

[34] S. SHERRIT, R. B. STIMPSON, H. D. WIEDERICK AND B.K. MUKHERJEE, Stress and Temperature

Dependence of the Direct Piezoelectric Charge Coefficient in Lead Zirconate Titanate Ceramics, SPIE Far

East and Pacific Rim Symposium on Smart Materials, 3321 (1996), pp. 74-81.

22

[35] H. H. A. KRUEGER AND D. BERLINCOURT, Effects of High Static Stress on the Piezoelectric Properties

of Transducer Materials, Journal of the Acoustical Society of America, 33, No. 10 (1961), pp. 1339-1344.

[36] The Piezo Book, Burleigh Instruments Inc., Piezo 330 692, Manufacturer Handbook, 14 pp.

[37] S. C. STEIN, C. LIANG AND C. A. ROGERS, Power consumption of piezoelectric actuators driving a

simply supported beam considering fluid coupling, J. of the Acoustical Society of America, 96 (1994), pp.

1598-1604.

[38] C. LIANG, F. P. SUN AND C. A. ROGERS, Coupled Electro-Mechanical Analysis of Adaptive Material

Systems-Determination of the Actuator Power Consumption and System Energy Transfer, J. of Intelligent

Mater. Syst. and Struct., 5 (1994), pp. 12-20.

[39] ANSYS/Multiphysics software, ANSYS, Inc. Southpointe 275 Technology Drive, Canonsburg, PA 15317.

[40] Y. KAGAWA AND T. YAMABUCHI, Finite Element Simulation of Two-Dimensional Electromechanical

Resonators, IEEE Trans. Sonics Ultrason., SU-21 (1974), pp. 275-283.

[41] R. LERCH, Modern Techniques in Electroacoustic Transducer Development, Proc. 9th Conf. Acoustics,

Budapest, Hungary, 1988.

[42] D. F. OSTERGAARD AND T. P. PAWLAK, Three-dimensional Finite Elements for Analysing Piezoelectric

Structures, Proc. IEEE Ultrason. Symp., Williamsburg, VA, pp. 639-642, 1986.

[43] R. LERCH, Simulation of Piezoelectric Devices by Two- and Three-Dimensional Finite Elements, IEEE

Transactions on Ultrasonics, Ferroelectrics, and Frequency Control, 37, No. 2 (1990), pp. 233 –247.

[44] R. SIMKOVICS, H. LANDES, M. KALTENBACHER AND R. LERCH, Nonlinear Finite Element Analysis

of Piezoelectric Transducers, IEEE Ultrasonics Symposium, pp. 1057-1060, 1999.

[45] R. PEREZ, E. MINGUELLA AND J. A. GORRI, Weak Nonlinearities in Piezoelectric Transducers:

Equivalent Circuits, Proceedings of the 11th IEEE International Symposium on Applications of

Ferroelectrics (ISAF), pp. 247 –250, 1998.

[46] M. OMURA, H. ADACHI AND Y. ISHIBASHI, Simulations of Ferroelectric Characteristics Using a One-

Dimensional Lattice Model, Japanese Journal of Applied Physics, 30 (1991), pp. 2384-2387.

[47] W. S. GALINAITIS AND R. C. ROGERS, Compensation for Hysteresis using Bivariate Preisach models,

SPIE Smart Structures and Materials: Mathematics and Control in Smart Materials, San Diego, CA, 1997.

[48] P.GE AND M. JOUANEH, Modeling Hysteresis in Piezoceramic Actuators, Precision Engineering, 17

(1995), pp. 211-221.

[49] X. D. ZHANG AND C. A. ROGERS, A Macroscopic Phenomenological Formulation for Coupled

Electromechanical Effects in Piezoelectricity, Journal of Intelligent Material Systems and Structures, 4

(1993), pp. 307-316.

[50] W. CHEN AND C. S. LYNCH, A Model for Simulating Polarization Switching and AF-F Phase Changes in

Ferroelectric Ceramics, Journal of Intelligent Material Systems and Structures, 9 (1998), pp. 427-431.

[51] R. C. SMITH AND Z. OUNAIES, A Domain Wall Model for Hysteresis in Piezoelectric Materials, Journal of

Intelligent Material Systems and Structures, 11, No. 1 (2000), p. 62.

[52] A.N. SOUKHOJAK, H. WANG, G.W. FARREY AND Y.-M. CHIANG, Superlattice in Single Crystal

Barium-Doped Sodium Bismuth Titanate, J. Phys. Chem. Solids, 61, No. 2 (2000), pp. 301-304.

Recommended